# Lecture Slides Chapter 2 Materials

## Presentation on theme: "Lecture Slides Chapter 2 Materials"— Presentation transcript:

Lecture Slides Chapter 2 Materials

Chapter Outline Shigley’s Mechanical Engineering Design

Shigley’s Mechanical Engineering Design

Used to obtain material characteristics and strengths
Standard Tensile Test Fig. 2–1 Used to obtain material characteristics and strengths Loaded in tension with slowly increasing P Load and deflection are recorded Shigley’s Mechanical Engineering Design

The stress is calculated from
Stress and Strain The stress is calculated from where is the original cross-sectional area. The normal strain is calculated from where l0 is the original gauge length and l is the current length corresponding to the current P. Shigley’s Mechanical Engineering Design

Stress-Strain Diagram
Plot stress vs. normal strain Typically linear relation until the proportional limit, pl No permanent deformation until the elastic limit, el Yield strength, Sy , defined at point where significant plastic deformation begins, or where permanent set reaches a fixed amount, usually 0.2% of the original gauge length Ultimate strength, Su , defined as the maximum stress on the diagram Ductile material Brittle material Fig. 2–2 Shigley’s Mechanical Engineering Design

Elastic Relationship of Stress and Strain
Slope of linear section is Young’s Modulus, or modulus of elasticity, E Hooke’s law E is relatively constant for a given type of material (e.g. steel, copper, aluminum) See Table A-5 for typical values Usually independent of heat treatment, carbon content, or alloying Fig. 2–2 (a) Shigley’s Mechanical Engineering Design

True Stress-Strain Diagram
Engineering stress-strain diagrams (commonly used) are based on original area. Area typically reduces under load, particularly during “necking” after point u. True stress is based on actual area corresponding to current P. True strain is the sum of the incremental elongations divided by the current gauge length at load P. Note that true stress continually increases all the way to fracture. Engineering stress-strain True Stress-strain (2-4) Shigley’s Mechanical Engineering Design

Compression tests are used to obtain compressive strengths.
Compression Strength Compression tests are used to obtain compressive strengths. Buckling and bulging can be problematic. For ductile materials, compressive strengths are usually about the same as tensile strengths, Suc = Sut . For brittle materials, compressive strengths, Suc , are often greater than tensile strengths, Sut . Shigley’s Mechanical Engineering Design

Torsional Strengths Torsional strengths are found by twisting solid circular bars. Results are plotted as a torque-twist diagram. Shear stresses in the specimen are linear with respect to the radial location – zero at the center and maximum at the outer radius. Maximum shear stress is related to the angle of twist by q is the angle of twist (in radians) r is the radius of the bar l0 is the gauge length G is the material stiffness property called the shear modulus or modulus of rigidity. Shigley’s Mechanical Engineering Design

Maximum shear stress is related to the applied torque by
Torsional Strengths Maximum shear stress is related to the applied torque by J is the polar second moment of area of the cross section For round cross section, Torsional yield strength, Ssy corresponds to the maximum shear stress at the point where the torque-twist diagram becomes significantly non-linear Modulus of rupture, Ssu corresponds to the torque Tu at the maximum point on the torque-twist diagram Shigley’s Mechanical Engineering Design

Modulus of resilience, uR
Resilience – Capacity of a material to absorb energy within its elastic range Modulus of resilience, uR Energy absorbed per unit volume without permanent deformation Equals the area under the stress- strain curve up to the elastic limit Elastic limit often approximated by yield point Shigley’s Mechanical Engineering Design

Area under curve to yield point gives approximation
Resilience Area under curve to yield point gives approximation If elastic region is linear, For two materials with the same yield strength, the less stiff material (lower E) has greater resilience Shigley’s Mechanical Engineering Design

Toughness – capacity of a material to absorb energy without fracture
Modulus of toughness, uT Energy absorbed per unit volume without fracture Equals area under the stress-strain curve up to the fracture point Shigley’s Mechanical Engineering Design

Area under curve up to fracture point
Toughness Area under curve up to fracture point Often estimated graphically from stress-strain data Approximated by using the average of yield and ultimate strengths and the strain at fracture Shigley’s Mechanical Engineering Design

Resilience and Toughness
Measures of energy absorbing characteristics of a material Units are energy per unit volume lbf·in/in3 or J/m3 Assumes low strain rates For higher strain rates, use impact methods (See Sec. 2-5) Shigley’s Mechanical Engineering Design

Statistical Significance of Material Properties
Strength values are obtained from testing many nominally identical specimens Strength, a material property, is distributional and thus statistical in nature Example – Histographic report for maximum stress of tensile tests on 1020 steel Shigley’s Mechanical Engineering Design

Example for Statistical Material Property
Histographic report for maximum stress of 1000 tensile tests on steel Probability density – number of occurrences divided by the total sample number Histogram of probability density for 1020 steel Fig. 2–5 Shigley’s Mechanical Engineering Design

Example for Statistical Material Property
Probability density function (See Ex. 20-4) Fig. 2–5 Shigley’s Mechanical Engineering Design

Standard deviation = 2.594 kpsi Distribution is normal Notated as
Statistical Quantity Statistical quantity described by mean, standard deviation, and distribution type From 1020 steel example: Mean stress = kpsi Standard deviation = kpsi Distribution is normal Notated as Shigley’s Mechanical Engineering Design

Property tables often only report a single value for a strength term
Strengths from Tables Property tables often only report a single value for a strength term Important to check if it is mean, minimum, or some percentile Common to use 99% minimum strength, indicating 99% of the samples exceed the reported value Shigley’s Mechanical Engineering Design

Cold Work Cold work – Process of plastic straining below recrystallization temperature in the plastic region of the stress-strain diagram Loading to point i beyond the yield point, then unloading, causes permanent plastic deformation, ϵp Reloading to point i behaves elastically all the way to i, with additional elastic strain ϵe Fig. 2–6 (a) Shigley’s Mechanical Engineering Design

The yield point is effectively increased to point i
Cold Work The yield point is effectively increased to point i Material is said to have been cold worked, or strain hardened Material is less ductile (more brittle) since the plastic zone between yield strength and ultimate strength is reduced Repeated strain hardening can lead to brittle failure Fig. 2–6 (a) Shigley’s Mechanical Engineering Design

Plot load P vs. Area Reduction
Reduction in Area Plot load P vs. Area Reduction Reduction in area corresponding to load Pf at fracture is R is a measure of ductility Ductility represents the ability of a material to absorb overloads and to be cold-worked (2-12) Fig. 2–6 (b) Shigley’s Mechanical Engineering Design

Cold-work factor W – A measure of the quantity of cold work
Fig. 2–6 (b) Shigley’s Mechanical Engineering Design

Equations for Cold-worked Strengths
Shigley’s Mechanical Engineering Design

Example 2-1 Shigley’s Mechanical Engineering Design

Example 2-1 (Continued) Shigley’s Mechanical Engineering Design

Two most common hardness-measuring systems Rockwell A, B, and C scales
Hardness – The resistance of a material to penetration by a pointed tool Two most common hardness-measuring systems Rockwell A, B, and C scales Specified indenters and loads for each scale Hardness numbers are relative Brinell Hardness number HB is the applied load divided by the spherical surface area of the indentation Shigley’s Mechanical Engineering Design

Strength and Hardness For many materials, relationship between ultimate strength and Brinell hardness number is roughly linear For steels For cast iron Shigley’s Mechanical Engineering Design

Example 2-2 Shigley’s Mechanical Engineering Design

Specimen struck by pendulum
Impact Properties Charpy notched-bar test used to determine brittleness and impact strength Specimen struck by pendulum Energy absorbed, called impact value, is computed from height of swing after fracture Shigley’s Mechanical Engineering Design

Effect of Temperature on Impact
Some materials experience a sharp transition from ductile to brittle at a certain temperature Fig. 2–7 Shigley’s Mechanical Engineering Design

Effect of Strain Rate on Impact
Average strain rate for stress-strain diagram is in/(in·s) Increasing strain rate increases strengths Due to yield strength approaching ultimate strength, a mild steel could be expected to behave elastically through practically its entire strength range under impact conditions Fig. 2–8 Shigley’s Mechanical Engineering Design

Temperature Effects on Strengths
Plot of strength vs. temperature for carbon and alloy steels As temperature increases above room temperature Sut increase slightly, then decreases significantly Sy decreases continuously Results in increased ductility Fig. 2–9 Shigley’s Mechanical Engineering Design

Often exhibits three stages
Creep Creep – a continuous deformation under load for long periods of time at elevated temperatures Often exhibits three stages 1st stage: elastic and plastic deformation; decreasing creep rate due to strain hardening 2nd stage: constant minimum creep rate caused by the annealing effect 3rd stage: considerable reduction in area; increased true stress; higher creep rate leading to fracture Fig. 2–10 Shigley’s Mechanical Engineering Design

Material Numbering Systems
Common numbering systems Society of Automotive Engineers (SAE) American Iron and Steel Institute (AISI) Unified Numbering System (UNS) American Society for Testing and Materials (ASTM) for cast irons Shigley’s Mechanical Engineering Design

UNS system established by SAE in 1975
UNS Numbering System UNS system established by SAE in 1975 Letter prefix followed by 5 digit number Letter prefix designates material class G – carbon and alloy steel A – Aluminum alloy C – Copper-based alloy S – Stainless or corrosion-resistant steel Shigley’s Mechanical Engineering Design

For steel, letter prefix is G
UNS for Steels For steel, letter prefix is G First two numbers indicate composition, excluding carbon content Second pair of numbers indicates carbon content in hundredths of a percent by weight Fifth number is used for special situations Example: G52986 is chromium alloy with 0.98% carbon Shigley’s Mechanical Engineering Design

Some Casting Processes
Sand Casting Shell Molding Investment Casting Powder-Metallurgy Process Shigley’s Mechanical Engineering Design

Hot-working Processes
Process in which metal is formed while heated above recrystallization temperature Refined grain size Rough surface finish Rolling, forging, extrusion, pressing Common bar cross-sections from hot-rolling Fig. 2–11 Shigley’s Mechanical Engineering Design

Cold-working Processes
Forming of metal without elevating temperature Strain hardens, resulting in increase in yield strength Increases hardness and ultimate strength, decreases ductility Produces bright, smooth, reasonably accurate finish Cold-rolling used to produce wide flats and sheets Cold-drawing draws a hot-rolled bar through a smaller die Fig. 2–12 Shigley’s Mechanical Engineering Design

Heat Treatment of Steel
Time and temperature controlled processes that modifies material properties Annealing Heated above critical temperature, held, then slowly cooled Refines grain structure, softens, increases ductility Erases memory of prior operations Normalizing provides partial annealing by adjusting time and temperature Quenching Controlled cooling rate prevents full annealing Less pearlite, more martensite and/or bainite Increased strength, hardness, brittleness Shigley’s Mechanical Engineering Design

Heat Treatment of Steel
Tempering Reheat after quenching to a temperature below the critical temperature Relieves internal stresses Increases ductility, slight reduction in strength and hardness Shigley’s Mechanical Engineering Design

Effects of Heat Treating
Fig. 2–13 Shigley’s Mechanical Engineering Design

Case Hardening Process to increase hardness on outer surface, while retaining ductility and toughness in the core Addition of carbon to outer surface by exposure to high carbon solid, liquid, or gas at elevated temperature Can also achieve case hardening by heat treating only the outer surface, e.g. induction hardening or flame hardening Shigley’s Mechanical Engineering Design

Alloy Steels Chromium Nickel Manganese Silicon Molybdenum Vanadium
Tungsten Shigley’s Mechanical Engineering Design

Corrosion-Resistant Steels
Stainless steels Iron-base alloys with at least 12 % chromium Resists many corrosive conditions Four types of stainless steels Ferritic chromium Austenitic chromium-nickel Martensitic Precipitation-hardenable Shigley’s Mechanical Engineering Design

Ductile and Nodular Cast Iron White Cast Iron Malleable Cast Iron
Casting Materials Gray Cast Iron Ductile and Nodular Cast Iron White Cast Iron Malleable Cast Iron Alloy Cast Iron Cast Steel Shigley’s Mechanical Engineering Design

Nonferrous Metals Aluminum Magnesium Titanium Copper-based alloys
Brass with 5 to 15 percent zinc Gilding brass, commercial bronze, red brass Brass with 20 to 36 percent zinc Low brass, cartridge brass, yellow brass Low-leaded brass, high-leaded brass (engraver’s brass), free-cutting brass Admiralty metal Aluminum brass Brass with 36 to 40 percent zinc Muntz metal, naval brass Bronze Silcon bronze, phosphor bronze, aluminum bronze, beryllium bronze Shigley’s Mechanical Engineering Design

Plastics Thermoplastic – any plastic that flows or is moldable when heat is applied Thermoset – a plastic for which the polymerization process is finished in a hot molding press where the plastic is liquefied under pressure Shigley’s Mechanical Engineering Design

Thermoplastic Properties (Table 2-2)
Shigley’s Mechanical Engineering Design

Thermoset Properties (Table 2-3)
Shigley’s Mechanical Engineering Design

Materials remain distinct from each other at the macroscopic level
Composite Materials Formed from two or more dissimilar materials, each of which contributes to the final properties Materials remain distinct from each other at the macroscopic level Usually amorphous and non-isotropic Often consists of laminates of filler to provide stiffness and strength and a matrix to hold the material together Common filler types: Fig. 2–14 Shigley’s Mechanical Engineering Design

Material Families and Classes (Table 2-4)
Shigley’s Mechanical Engineering Design

Material Families and Classes (Table 2-4)
Shigley’s Mechanical Engineering Design

Material Families and Classes (Table 2-4)
Shigley’s Mechanical Engineering Design

Material Families and Classes (Table 2-4)
Shigley’s Mechanical Engineering Design

Young’s Modulus for Various Materials
Fig. 2–15 Shigley’s Mechanical Engineering Design

Young’s Modulus vs. Density
Fig. 2–16 Shigley’s Mechanical Engineering Design

Specific Modulus – ratio of Young’s modulus to density, E / r
Also called specific stiffness Useful to minimize weight with primary design limitation of deflection, stiffness, or natural frequency Parallel lines representing different values of E / r allow comparison of specific modulus between materials Fig. 2–16 Shigley’s Mechanical Engineering Design

Minimum Mass Guidelines for Young’s Modulus-Density Plot
Guidelines plot constant values of Eb/r b depends on type of loading b = 1 for axial b = 1/2 for bending Example, for axial loading, k = AE/l  A = kl/E m = Al = (kl/E) l =kl2  /E Thus, to minimize mass, maximize E/ ( = 1) Fig. 2–16 Shigley’s Mechanical Engineering Design

The Performance Metric
The performance metric depends on (1) the functional requirements, (2) the geometry, and (3) the material properties. The function is often separable, f3 (M) is called the material efficiency coefficient. Maximizing or minimizing f3 (M) allows the material choice to be used to optimize P. Shigley’s Mechanical Engineering Design

Performance Metric Example
Requirements: light, stiff, end-loaded cantilever beam with circular cross section Mass m of the beam is chosen as the performance metric to minimize Stiffness is functional requirement Stiffness is related to material and geometry Shigley’s Mechanical Engineering Design

Performance Metric Example
From beam deflection table, Sub Eq. (2-26) into Eq. (2-25) and solve for A The performance metric is Sub Eq. (2-27) into Eq. (2-28), Shigley’s Mechanical Engineering Design

Performance Metric Example
Separating into the form of Eq. (2-24), To minimize m, need to minimize f3 (M), or maximize Shigley’s Mechanical Engineering Design

Performance Metric Example
M is called material index For this example, b = ½ Use guidelines parallel to E1/2/r Increasing M, move up and to the left Good candidates for this example are certain woods, composites, and ceramics Fig. 2–17 Shigley’s Mechanical Engineering Design

Performance Metric Example
Additional constraints can be added as needed For example, if it is desired that E > 50 GPa, add horizontal line to limit the solution space Wood is eliminated as a viable option Fig. 2–18 Shigley’s Mechanical Engineering Design

Strength vs. Density Fig. 2–19 Shigley’s Mechanical Engineering Design

Specific Strength – ratio of strength to density, S / r
Specific Modulus Specific Strength – ratio of strength to density, S / r Useful to minimize weight with primary design limitation of strength Parallel lines representing different values of S / r allow comparison of specific strength between materials Fig. 2–19 Shigley’s Mechanical Engineering Design

Minimum Mass Guidelines for Strength-Density Plot
Guidelines plot constant values of Sb/r b depends on type of loading b = 1 for axial b = 2/3 for bending Example, for axial loading,  = F/A = S  A = F/S m = Al = (F/S) l Thus, to minimize m, maximize S/ ( = 1) Fig. 2–19 Shigley’s Mechanical Engineering Design